| ||Format||Pages||Price|| |
|16||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||16||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||32||$62.40||  ADD TO CART|
Significance and Use
5.1 The test temperature for this test is related to the temperature experienced by the pavement in the geographical area for which the asphalt binder is intended to be used.
5.2 The complex shear modulus is an indicator of the stiffness or resistance of asphalt binder to deformation under load. The complex shear modulus and the phase angle define the resistance to shear deformation of the asphalt binder in the linear viscoelastic region. The complex modulus and the phase angle are used to calculate performance-related criteria in accordance with Specification or AASHTO Standard M320.
1.1 This test method covers the determination of the dynamic shear modulus and phase angle of asphalt binders when tested in dynamic (oscillatory) shear using parallel plate geometry. It is applicable to asphalt binders having dynamic shear modulus values in the range from 100 Pa to 10 MPa. This range in modulus is typically obtained between 4 and 88°C at 10 rad/s. This test method is intended for determining the linear viscoelastic properties of asphalt binders as required for specification testing and is not intended as a comprehensive procedure for the full characterization of the viscoelastic properties of asphalt binders.
1.2 This standard is appropriate for unaged materials, material aged in accordance with Test Method , material aged in accordance with Practice , or material aged in accordance with both Test Method and Practice . This procedure is limited to asphalt binders that contain particles with largest dimension less than 250 μm.
1.3 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.4 This standard may involve hazardous materials, operations, and equipment. This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials
D140 Practice for Sampling Bituminous Materials
D2170 Test Method for Kinematic Viscosity of Asphalts (Bitumens)
D2171 Test Method for Viscosity of Asphalts by Vacuum Capillary Viscometer
D2872 Test Method for Effect of Heat and Air on a Moving Film of Asphalt (Rolling Thin-Film Oven Test)
D6373 Specification for Performance Graded Asphalt Binder
D6521 Practice for Accelerated Aging of Asphalt Binder Using a Pressurized Aging Vessel (PAV)
E77 Test Method for Inspection and Verification of Thermometers
E563 Practice for Preparation and Use of an Ice-Point Bath as a Reference Temperature
E644 Test Methods for Testing Industrial Resistance Thermometers
E882 Guide for Accountability and Quality Control in the Chemical Analysis Laboratory
Deutsche Industrie Norm (DIN) Standard43760 Standard for Calibration of Thermocouples
AASHTO StandardsM320 Standard Specification for Performance-Graded Asphalt Binder T315
ICS Number Code 93.080.20 (Road construction materials)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D7175-15, Standard Test Method for Determining the Rheological Properties of Asphalt Binder Using a Dynamic Shear Rheometer, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top